Template-free electrodeposition of case.edu/cse/eche/daigroup/Journal...
Embed Size (px)
Transcript of Template-free electrodeposition of case.edu/cse/eche/daigroup/Journal...
Template-free electrodeposition of multicomponent metal nanoparticles for region-specific
growth of interposed carbon nanotube micropatterns
This article has been downloaded from IOPscience. Please scroll down to see the full text article.
2005 Nanotechnology 16 2111
IP Address: 188.8.131.52
The article was downloaded on 02/04/2012 at 14:29
Please note that terms and conditions apply.
View the table of contents for this issue, or go to the journal homepage for more
Home Search Collections Journals About Contact us My IOPscience
INSTITUTE OF PHYSICS PUBLISHING NANOTECHNOLOGY
Nanotechnology 16 (2005) 21112117 doi:10.1088/0957-4484/16/10/023
Template-free electrodeposition ofmulticomponent metal nanoparticles forregion-specific growth of interposedcarbon nanotube micropatternsLingchuan Li and Liming Dai1
Department of Chemical and Materials Engineering, School of Engineering and UDRI,University of Dayton, 300 College Park, Dayton, OH 45469-0240, USA
Received 19 May 2005, in final form 27 June 2005Published 9 August 2005Online at stacks.iop.org/Nano/16/2111
AbstractWe have demonstrated that multicomponent carbon nanotube micropatterns,in which different nanotubes are interposed in an intimate fashion, can beprepared by pyrolytic growth of carbon nanotubes on interposedmicropatterns of different metal nanoparticles generated by template-freepulsed electrodeposition of metal-containing salts onto aphotolithographically prepatterned conductive surface at different peakpotentials. The resultant multicomponent interposed carbon nanotubemicropatterns should have important implications for the construction ofmulticomponent and multifunctional nanomaterials and nanodevices basedon carbon nanotubes for a wide range of potential applications.
(Some figures in this article are in colour only in the electronic version)
With the recent significant advances in nanoscience andnanotechnology, various nanostructured metals and metalalloys have been prepared for a wide range of potentialapplications. Examples include the use of metal nanoparticlesas advanced catalysts and metal nanowires as efficient electronemitters [1, 2]. In particular, a large number of techniques,including the vapour deposition of metal thin films coupledwith annealing in a reducing atmosphere , wet depositionof dilute solutions of metal salts followed by calcinations andannealing in reducing atmosphere , direct inclusion ofmetal nanoparticles in colloid suspension  or solgelsystems [20, 21], and plasma etching or ion bombardment ofmetallic substrates [22, 23], have been devised for preparingmetal nanocatalysts on substrates for carbon nanotube growth.Although the electroplating of metals on conductive substrateshas a long history in industrial applications, only a few recentstudies involve the use of electrodeposited metals, mainly in the
1 Author to whom any correspondence should be addressed.
nanopores of alumina template membranes, to produce metalnanoparticles for the growth of carbon nanotubes .In these cases, a rather tedious post-synthesis process isoften required to remove the template to produce pure carbonnanotubes .
On the other hand, carbon nanotubes have been demon-strated to be useful in many microscale or nanoscale electronicand photonic devices . The ability to manipulate themfor heterogeneous integration on a micrometre to nanometrescale is of paramount importance to both fundamental char-acterization and potential applications of carbon nanotubesin various advanced optoelectronic devices [28, 29]. In thiscontext, we have developed microfabrication methods for mi-cropatterning of carbon nanotubes with a submicrometre res-olution . Following our earlier work on the micro-fabrication of carbon nanotubes, we have recently carried outthe template-free electrodeposition of cobalt (nickel) nanopar-ticles by applying an AC voltage across an aluminium work-ing electrode and graphite (nickel foil) counter-electrode in atwo-electrode electrochemical cell containing an aqueous so-lution of 0.4 M H3BO3 and 0.3 M CoSO4 (0.3 M NiSO4).
0957-4484/05/102111+07$30.00 2005 IOP Publishing Ltd Printed in the UK 2111
L Li and L Dai
The resultant metal nanoparticles with a nanometre-scale size,together with the ease with which multicomponent inter-posed metal nanoparticle micropatterns could be prepared by aregion-specific template-free electroplating, prompt us to growinterposed multicomponent micropatterns of different carbonnanotubes from the interposed micropatterns of different metalnanoparticles. Here, we report this simple, but very effec-tive, template-free electroplating method for region-specificdeposition of cobalt and nickel nanoparticles for patternedgrowth of carbon nanotubes. The resulting carbon nanotubemicropatterns in which multicomponents are interposed in acontrollable fashion should be of significance for manynanotube-based multifunctional systems, such as sensor chipsand multifunctional optoelectronic devices .
2. Experimental details
2.1. Materials and characterization
Aluminium foils were cut into pieces of 12 mm 60 mmas the electrodes. H3BO3, NiSO4 and CoSO4 were allanalytical grade, purchased from commercial sources and usedwithout further purification. Positive photoresist AZ 3312and the corresponding AZ 300 MIF developer were suppliedby Clariant Corporation. A medium pressure mercury UVlamp and TEM copper grids of both 200 and 600 mesheswere used as the UV light and photomask, respectively, forphotopattering. Scanning electron microscopic (SEM) imageswere recorded on a Hitachi S-2150 SEM unit and a Hitachi S-900 field emission-type SEM unit. Atomic force microscope(AFM) images were taken with a Digital Instruments AFM(Veeco Metrology), using the tapping mode.
2.2. Patterned and nonpatterned electrodepositions
Prior to the electrodeposition, the aluminium surface wascleaned in an aqueous solution of chromic acid (2 wt%),phosphoric acid (6 wt%) and hydrofluoric acid (0.001 wt%).The aluminium electrodes were then electropolished in amixture of perchloric acid and alcohol; this was followedby electrodeposition of nickel and cobalt nanoparticles inaqueous solutions of 0.4 M H3BO3/0.3 M NiSO4 and 0.4 MH3BO3/0.3 M CoSO4, respectively. Figure 1 shows thesteps of the patterned electrodeposition of nickel and cobaltnanoparticles. Prior to the patterned electrodeposition ofmetal nanoparticles, a thin layer of positive photoresist(AZ 3312 from Clariant Corporation) was spin-cast on theelectropolished aluminium surface; this was followed bydrying in an oven at 80 C. Upon UV exposure from a mediumpressure mercury lamp through a TEM grid as the photomask,the photoresist film in the exposed regions was renderedsoluble in AZ 300 MIF developer purchased from the samecompany. Cobalt nanoparticles were then electrochemicallydeposited into the photoresist-free areas within the patternedphotoresist structure under an alternating potential (60 Hz) of6.5 V with a graphite rod counter-electrode in an aqueoussolution of 0.4 M H3BO3 and 0.3 M CoSO4 for 20 s. Thenewly formed cobalt nanoparticles were then stabilized andpreserved by immersing the electrodeposited sample into a 5%potassium dichromate solution. Subsequent washing of the
(i) Photoresist application
(ii) UV exposure
(iv) Co electrodeposition
(v) Photoresist removal
(vi) Ni electrodeposition
Figure 1. Schematic representation of the region-specificelectrodeposition of cobalt and nickel nanoparticles.
cobalt-deposited electrode with flowing water and anhydrousacetone removed the resist that was not exposed to the UVlight to regenerate the underlying aluminium surface. Afterbeing cleaned again by immersing in a dilute solution ofsodium hydroxide and potassium dichromate for a few secondsthis time, the resulting electrode prepatterned with cobaltnanoparticles was then used for electrodeposition of nickelnanoparticles at 4.0 V with the alternating power and a nickelfoil counter-electrode in an aqueous solution of 0.4 M H3BO3and 0.3 M NiSO4 for 1 min. As cobalt and nickel nanoparticleswere electrodeposited under two different voltages, the highvoltage (AC 6.5 V) applied during the cobalt deposition couldlead to the formation of a relatively thick charge barrier layerby electro-oxidation of aluminium at the negative half-cycleof the alternating potential, which can act as an effectiveinsulating coating at the relatively low voltage required for thenickel deposition (AC 4.0 V) to avoid the formation of nickelnanoparticles over the cobalt-covered areas. As we shall seelater, a desired particle size and packing density for nanotubegrowth make 20 s and 1 min the electrodeposition times ofchoice for Co and Ni, respectively.
Template-free electrodeposition of multicomponent metal nanoparticles
Figure 2. SEM images of (a) an aluminium surface after electropolishing (see section 2), (b) after the template-free electrodeposition ofnickel particles at 4.0 V for 5 s; AFM images of (c) the nickel nanoparticles